Uncovering the mystery of ferroelectricity in zero dimensional nanoparticles

It is generally accepted that chemically synthesized nanoparticles lose their ferroelectricity (spontaneous polarization) as the particles become smaller. In contrast, ball-milled ferroelectric nanoparticles have an enhanced ferroelectric response at remarkably small sizes (≤10 nm). Although prior theory suggests that surface stress influences ferroelectricity, the source of such a stress and how it physically influences ferroelectricity in zero-dimensional nanoparticles has remained a mystery. In this paper, we demonstrate that the top-down approach of wet ball-milling not only results in fragmented materials on the nanoscale, but it also is responsible for a mechanochemical synthesis of metal carboxylates forming at the nanoparticles' surface. We prove that the presence of such a compound with a particular type of binding mode chemisorbed at the nanoparticles' surface is responsible for producing surface stress. This surface stress results in a stabilization and dramatic enhancement of the spontaneous polarization, which is 5 times greater than that of the bulk material and 650 times greater than what is measured in materials fabricated using standard chemical synthesis techniques. The results of this study have further led to the development of a new process that produces ferroelectric nanoparticles (≤10 nm) with uniform shape and size using a combination of wet chemistry and mechanochemical synthesis.


Introduction
It has been well-documented in the literature that the spontaneous polarization/dipole moment dramatically reduces in magnitude as the particle/grain size of conventional ferroelectrics becomes less than 100 nm. 1 However, there have been several papers on the discovery of ferroelectricity in BaTiO 3 nanocolloids/nanoparticles prepared by wet ball-milling in nonpolar heptane with oleic acid. These samples demonstrate very large values of spontaneous polarization; 2,3 this is in strong contradiction to what is observed in nanoparticles/nanograins produced via traditional wet chemistry routes and ceramic fabrication, i.e. solvothermal synthesis, sol-gel, spark plasma sintering, etc. 1,4,5 Although the physics of ball-milled ferroelectric nanoparticles has not been well understood, they have been widely used in liquid crystal studies over the past couple of decades showing remarkable enhancements of both electrical-and electro-optical responses. [6][7][8][9] Moreover, ball-milled ferroelectric nanoparticles have been used outside of optical/liquid crystal applications for molecular catalysis applications, where the large dipole eld from the ferroelectric nanoparticles replaces the need for any external bias. 10 Prior to this current paper, ball-milling was mainly considered as a simple top-down approach for fabricating randomly shaped ferroelectric nanoparticles, without a formal explanation for the existence of ferroelectricity on such a small scale. Since any observed ferroelectricity was extremely weak at best in chemically produced nanoparticles, opposed to the strong response detected in ball-milled nanoparticles, it was assumed that surface stress was mechanically-induced during the high energy ball-milling process. 2,11,12 Although theory in 2007 and experimental evidence in 2010 supported this claim, 2,11,12 it was only supposition that the high impact velocity of the milling beads could impart a surface stress in the particles during grinding. The exact mechanism for the creation of the stress that provided such a large spontaneous polarization was unknown. It was also believed that the oleic acid, a typical choice of surfactants, served solely as a means of preventing particle aggregation. 9,[12][13][14] However, a recent discovery in ref. 15 shows that ball-milling not only results in a top-down approach for the mechanical creation of ferroelectric nanoparticles, it also results in a chemical reaction at the nanoparticle surface (i.e. a mechanochemical formation of large quantities of barium oleate from the oleic acid starting material). With the conclusions drawn in ref. 15, a revision of this common point of view, that ball-milling only results in the fragmentation of the particles, is required.
In this paper, it is shown that a metal carboxylate bulk compound, resulting from mechanochemical synthesis, plays a key role in stabilizing/enhancing ferroelectricity in wet ballmilled nanoparticles. A relationship is established between the spontaneous polarization of these nanoparticles and their surface interactions with surrounding molecular entities. Evidence is presented proving that only a certain type of coordination binding mode of carboxylates possessing a molecular packing order/crystalline structure is chemisorbed at the nanoparticles' surface; this particular metal carboxylate is responsible for a surface stress and in turn a stabilization and dramatic enhancement of ferroelectricity (spontaneous polarization). The identication and explanation of the physical differences of the carboxylate functional groups and the types of coordination binding modes for both chemically (traditional wet chemistry approaches) and mechanically (ball-milling) produced nanoparticles is also investigated. Furthermore, a new technique/process is presented that overcomes the major drawback of ball-milled nanoparticles, i.e. their random shape. This new technique results in a controllable uniform shape and size of highly ferroelectric nanoparticles, whose properties are dened by the type of coordination binding mode of a barium oleate COO À carboxylate. The difference in the binding modes is what allows for the typical amorphous (quasi-bridging bidentate structure) organic coating to become a crystalline (chelate bidentate structure) "shell" as a result of mechanochemical synthesis. Finally, the physical mechanism enabling a surface stress and thus a ferroelectric stabilization and enhancement is determined for the rst time. The surface stress, which is shown in this work to be an epitaxial-like stress/ strain between the inorganic core and the surrounding crystalline organic component, is responsible for a 650 times (>130 mC cm À2 ) enhancement of the spontaneous polarization in BaTiO 3 nanoparticles compared to non-stressed BaTiO 3 nanoparticles; this is a 5 times increase compared to the value found in bulk BaTiO 3 (26 mC cm À2 ). The fundamental understanding of the surface physics and ability of its manipulation opens many doors for producing surface relevant properties for various applications, e.g. catalysis, liquid crystal displays, photorefractive beam coupling in hybrid devices, etc. [6][7][8][9][10]16 This discovery paves the road toward the creation and control of ferroelectricity in uniformly-shaped "zero dimensional" ferroelectric "superparticles", where the term superparticles (used in ref. 2) applies to this new class of nanoparticles where the spontaneous polarization belongs to the inorganic-organic hybrid core-shell system (core nanoparticle and functional shell) and not just the inorganic nanoparticle itself.

Background
It is widely accepted that ferroelectric materials undergo a degradation of their hallmark properties with size reduction, and even a complete disappearance at a critical size. 1,[17][18][19] This size dependence is manifested in the reduction of the Curie temperature, the diffusive character of the phase transition, and the suppression of the spontaneous polarization. Therefore, the current challenge in nanoscale ferroelectrics is to stabilize and enhance ferroelectricity, while reducing the materials' dimensionality. Depending on the dimensionality of the nanomaterial, either 2-D thin lms or 0-D nanoparticles, different strategies and mechanisms of ferroelectricity enhancement may be employed. Thin 2-D lm technologies have demonstrated a steady and tangible success with well-developed fabrication procedures and a deep understanding of the materials' physics. As such, Choi et al. employed an elastic strain engineering concept based on a lattice mismatch, achieving a 230% (60 mC cm À2 ) enhancement of the spontaneous polarization (compared to bulk BaTiO 3 , 26 mC cm À2 ) in epitaxially grown BaTiO 3 multilayered thin lms; 20 this is supported by Ederer et al. whose theory shows a linear dependence of the spontaneous polarization as a function of elastic strain. 21 A different scenario is considered for 0-D nanoparticles synthesized via conventional wet chemistry routes. The relaxing synthetic conditions set modalities for the growth of nanoparticles with paraelectric centrosymmetric structures, where the properties are mainly determined by the inorganic core of the nanoparticle with no functionality from a coating/shell. Numerous experimental works fall into this paradigm supported by the size dependent phenomenological Landau-Devonshire-Ginzburg (LDG) theory. 22,23 For instance, Caruntu et al. synthesized and characterized well-dened single domain BaTiO 3 nanocubes and nanospheres. 4,24 The value of spontaneous polarization of similar samples as found in ref. 4 (provided to us by G. Caruntu and measured in our laboratory) was 0.2 mC cm À2 (about 1% the value for the bulk crystal); the fact that these nanoparticles existed in the ferroelectric phase was an improvement to those that had been conned to the paraelectric phase.
Alternatively, a top-down approach (ball-milling) has been used to fabricate small BaTiO 3 nanoparticles (randomly-shaped), 2,3,7-10,12-15,25 which has revolutionized the eld by offering a simple and effective technique to create highly ferroelectric BaTiO 3 nanoparticles. Morozovska et al. proposed a mechanism for such an enhancement to be linked to surface stress/strain; 11 direct experimental proof of the presence of such a surface stress in randomly-shaped ball-milled BaTiO 3 nanoparticles with large spontaneous polarization values (100-120 mC cm À2 ) is demonstrated in ref. 2, 3 and 12, although the source of the stress remained a mystery.
To further improve the ferroelectric properties and overcome these fundamental limitations, it is necessary to explore novel mechanisms of enhancement by taking into consideration not only the nanoparticle core, but also its surface and interface. This current work identies and describes the source of surface stress, thus unraveling the mystery of the strong ferroelectric effect on a nanoscale (#10 nm); it also investigates functional surface bonds, unachievable by conventional chemistry, 26,27 which provide the required conditions for the enhancement of ferroelectric properties.

Synthesis of BaTiO 3 nanocolloids and their components
A series of materials were prepared using various methods: (1) ball-milled BaTiO 3 nanoparticles were prepared using commercial Aldrich powder as reported in ref. 2,8,9,12,13 and 15, (2) BaTiO 3 nanocubes (pre-milled) were created using solvothermal synthesis following the method used in ref. 4, and (3) post-milled BaTiO 3 nanocubes were prepared by ball-milling the nanocubes obtained in (2) using a planetary high energy ball-mill Retsch PM 100. For this latter case, a slurry comprising 0.1 g of synthesized BaTiO 3 nanocubes, 0.1 g of oleic acid and 15 ml of heptane was immersed into a ball-mill crucible lled with 2 mm ZrO 2 beads and subjected to rotation at 500 rpm for 5 hours; the produced nanoparticles/nanocubes were converted to powder using anhydrous ethanol with sequential washing/ drying at ambient temperature, resulting in a white precipitate. All starting materials included oleic acid unless noted otherwise. Note: the use of the term nanocubes refers to nanoparticles with a controlled cubic shape achieved using the solvothermal synthesis technique. The same milling conditions were also used for the creation of ball-milled BaTiO 3 nanoparticles of random shape in (1) using a precursor BaTiO 3 powder supplied by Aldrich. Individual components of ballmilled commercial barium oleate (Pfaltz & Bower), and unmilled commercial BaTiO 3 (Aldrich) powder were also investigated.

Characterization of BaTiO 3 nanoparticles
Optical, electrical, and morphological studies were performed on the above-mentioned nanomaterials. Temperature dependent infrared (IR) absorption spectra were measured using Fourier-transform infrared spectroscopy with an FTIR-NIR Bruker spectrophotometer in an Attenuated Total Reection (ATR) conguration over the range of 400-3000 cm À1 with 2 cm À1 resolution. AC displacement current density measurements, as described in ref. 2, 3 and 10, provided values of the spontaneous polarization of samples that were diluted (1 : 1000) with heptane containing 0.4% by weight of oleic acid. Surface morphology was investigated using a Philips CM 200 transmission electron microscope with 200 kV accelerating voltage. In addition, X-ray diffraction (XRD) measurements were conducted on dried out solutions of samples ball-milled in heptane with oleic acid (weight ratio of oleic acid : BaTiO 3 was 1 : 1) and without oleic acid, as well as ball-milled commercial barium oleate and commercial BaTiO 3 starting powders. Thermogravimetric analysis (TGA) measurements were conducted to verify the organic phase of the core-shell nanoparticles using a TA Instruments Q500 TGA.

Results and discussion
To explore the effects responsible for the ferroelectric stabilization and enhancement and provide empirical evidence to support these claims, several samples were studied. These samples are referred to throughout the text as: "ball-milled nanoparticles" (using commercial starting materials, Aldrich powder), "pre-milled nanocubes" (produced by solvothermal synthesis following the recipe from ref. 4), "post-milled nanocubes" (solvothermal synthesized nanocubes subjected to postgrowth high-energy ball-milling as a means of mechanochemical synthesis), and "ball-milled commercial barium oleate".
The identication of both the local structure of barium oleate and the long-range molecular ordering can be achieved using FTIR spectroscopy. 28 Fig. 1 shows the FTIR absorption spectra for: ball-milled commercial barium oleate, ball-milled BaTiO 3 nanoparticles, pre-milled BaTiO 3 nanocubes, and postmilled BaTiO 3 nanocubes. Note, the average nanoparticle size reduces as the milling time increases, asymptotically reaching a minimum average size of approximately 9-10 nm. 9,13 For this reason ball-milling of the solvothermal synthesized $10 nm nanocubes was not expected to reduce the size any further, although it was expected that it could affect the chemical properties of the organic component (coating/shell) and the level of surface stress. Note: the surrounding organic material coating the nanoparticle will be referred to as a "shell" for the remainder of this paper. TEM images of synthesized BaTiO 3 nanocubes are shown in Fig. 1 for both the pre-milled and the post-milled material. There is no signicant change in the average size or shape of the pre-and post-milled nanocubes; this is a dramatic improvement in uniformity over the top-down approach of ball-milling bulk material (see ref. 13 and 14), which did not allow for any control of the shape of the nanoparticles.
In Fig. 1, the FTIR absorption spectra of (a), (b) and (d) are nearly identical with only minor differences, such as the feature centered around 1710 cm À1 and the low-frequency tail. The 1710 cm À1 absorption band is a "ngerprint" of the vibrational mode of carbonyl (C]O), which is associated with the presence of free oleic acid molecules found in commercial barium oleate, and the broad low-frequency tail is due to the BaTiO 3 absorption. The spectrum of the pre-milled BaTiO 3 nanocubes (Fig. 1c) is distinctly different from the others suggesting a different type of COO À coordination binding mode. It is known for different types of carboxylates, that the splitting in energy between asymmetrical and symmetrical stretching vibrations (u asym À u sym ¼ D) is indicative of the type of carboxylate coordination binding mode. 29,30 Based on this criteria, the four major carboxylate structures can be characterized as follows (see Fig. 2): 30,31 (I) D > 110 cm À1a bridging bidentate, in which each oxygen of the carboxylate covalently bonds to a different metal cation; (II) D < 110 cm À1a chelating bidentate, in which charge of the carboxylate is shared across the oxygen atoms, and both form covalent bonds with the metal cation; (III) D > 200 cm À1a covalent monodentate, in which a negatively charged oxygen of the carboxylate forms a covalent bond with the metal ion; and (IV) an ionic monodentate, in which one negatively charged oxygen of the carboxylate and a metal cation form an ionic bond. Typically, the characteristic IR absorption bands for metal carboxylates, in particularly the carboxylate group (COO À ), are in the range 1500-1610 cm À1 for asymmetrical stretching modes (u 1 in Fig. 1) and 1300-1450 cm À1 for symmetrical stretching modes (u 2 in Fig. 1). For the samples shown in Fig. 1a, b and d, the sharp absorption band at 1510 cm À1 and the shoulder around 1540 cm À1 are related to asymmetrical stretching modes, while the 1408 cm À1 band is related to the symmetrical stretching modes. The 1466 cm À1 band is assigned as a CH 2 bend (d (CH 2 ) scissoring band), 29 however, an assignment of 1433 cm À1 is not straightforward. It may be related to symmetrical stretching such that there are two pairs of u asym and u sym frequencies (u asym ¼ 1510 cm À1 , u sym ¼ 1408 cm À1 and u asym ¼ 1540 cm À1 , u sym ¼ 1433 cm À1 ) with a value of D for both cases being <110 cm À1 , justifying the chelate structure (Fig. 2, type II). On the other hand, the 1433 cm À1 feature may be related to CH 2 vibrations resulting from the overlap of u 1 (COO À ) stretching and d (CH 2 ) scissoring bands. In this case, a mixture of both chelate and quasibridging (D value for the pair 1540 cm À1 and 1408 cm À1 is 132 cm À1 ) coordination binding modes would need to be considered. Nevertheless, the presence of a chelate structure is dominating in these samples (for example, see the 1510 cm À1 strong absorption in the cases of Fig. 1a, b and d); this type of local structure favors an ordered arrangement of barium oleate molecules at the nanoparticle surface. Equally spaced absorption bands in the range 1180-1350 cm À1 (progressive bandsattributed to wagging/twisting vibrations of chains of successive methylene groups of the barium oleate molecule) and the 720 cm À1 feature (attributed to rocking vibrations of chains of successive methylene groups of the barium oleate molecule) both serve as proof of crystallization of barium oleate. [29][30][31] This claim is supported by the work of Koga and Matuura, 32 who extensively studied the relationship between FTIR absorption spectra and the structure of metal carboxylates. They showed that the type of carboxylate coordination can dictate the character of the molecular packing order, ranging from crystalline basalt to amorphous structures, which is the case for BaTiO 3 nanoparticles/nanocubes with oleate shells in chelate and quasi-bridging congurations, respectively. Further evidence of the crystalline structure of the chelate bidentate in the ballmilled samples is shown in the diffraction patterns of the XRD data found in Fig. 3.
The ball-milled sample with oleic acid presented in Fig. 3d is comprised of two phases: an organic phase of barium oleate (i.e. mechanochemical synthesis converted oleic acid to an ordered chelate-structured metal carboxylate, Fig. 2, type II) characterized by the equally spaced sharp diffraction peaks below 20 of 2q, and an inorganic phase of BaTiO 3 nanoparticles characterized by broad diffraction peaks above 20 of 2q. Individual milled organic and unmilled inorganic components are shown in Fig. 3b and c, respectively. Thermogravimetric analysis (TGA) measurements conrmed the presence of an organic phase in the sample and estimated its quantity to be at least 50% by weight, which is in agreement with the results using an independent method in ref. 15. It is worth noting that the sharp diffraction peaks below 20 of 2q in Fig. 3b and d demonstrate the crystalline nature of the organic component found in pure (ball-milled) barium oleate in an ordered chelate coordination binding mode and ball-milled BaTiO 3 (with oleic acid), respectively. It is worth emphasizing that two independent methods, FTIR and XRD, both demonstrate that milled nanoparticles/  nanocubes have crystalline organic shells, as opposed to the case of unmilled/pre-milled materials. For the case of the ballmilled BaTiO 3 without oleic acid in heptane, diffraction peaks from BaTiO 3 and barium oleate are not observed below 20 of 2q (Fig. 3a). The diffraction peak at $14 seen in Fig. 3a is not present in Fig. 3d. It is also worth noting that the absorption spectra of the samples used for Fig. 3a and c (no oleic acid in the starting material) do not resemble the spectra of the BaTiO 3 samples milled with oleic acid (data not shown). The sample used for Fig. 3d gives a very large spontaneous polarization (due to the presence of the metal carboxylate), unlike the sample used for Fig. 3a (which contains no metal carboxylates). We therefore conclude that the source of this feature at $14 does not play a role in the spontaneous polarization enhancement. The source responsible for this diffraction peak may have been formed as a byproduct of ball-milling BaTiO 3 in heptane (without oleic acid).
In contrast to the discussion above, the FTIR absorption spectrum of the pre-milled nanocubes in Fig. 1c shows broad asymmetrical stretching (centered at 1545 cm À1 with no sign of the 1510 cm À1 absorption band) and broad symmetrical stretching (centered at 1426 cm À1 including the 1408 cm À1 band) carboxylate modes with an energy splitting (D) of either 119 cm À1 or 137 cm À1 ; in both cases the D-values correspond to the quasi-bridging binding mode (Fig. 2, type I). This type of local structure favors a random (amorphous) distribution of barium oleate molecules at the nanoparticle (nanocube) surface, and therefore cannot provide a lattice mismatch between the shell and the core. The complete assignment of IR absorption lines of the samples is in Table 1. [28][29][30][31][32] Similar in nature to the transformation of the quasi-bridging to chelate coordination binding modes resulting from mechanochemical synthesis (i.e. high energy ball-milling), a transformation of the crystalline chelate bidentate to the amorphous quasi-bridging bidentate was observed by annealing the milled BaTiO 3 nanoparticles (milled Aldrich powder from Fig. 1b) at 140 C, which is above the Curie temperature. Fig. 4a-d show the FTIR absorption spectra of the ball-milled nanoparticles before annealing, and as a function of time at room temperature aer cooling. It can be seen that annealing the sample drastically modies the absorption spectrum, as shown in Fig. 4b (note, the spectra in Fig. 4b and f were measured 10 min aer cooling the sample to room temperature to provide a uniform temperature throughout the sample). In particular, the intensity of the 1540 cm À1 band increased at the expense of the 1510 cm À1 band, i.e. amorphous metal carboxylates increased at the expense of crystalline metal carboxylates, which was proven to be a reversible process in Fig. 4 as the sample with a time delay on the order of hours (Fig. 4d) showed nearly a full recovery of the 1510 cm À1 band (i.e. a reversal of the amorphous   quasi-bridging structure back to the crystalline chelate structure). This recongurable "self-healing" mechanism was observed only for samples that initially had the chelate structure. Unlike the reversible-nature of the oleate-shell surrounding the ball-milled nanoparticles, the annealing of milled commercial barium oleate resulted in a permanent transformation of the sample's bond structure to a quasibridging coordination binding mode with a broadening of asymmetrical and symmetrical absorption bands, shown in Fig. 4e-g. A key observation is the similarity between Fig. 1c and 4b, where the pre-milled nanocubes (with the type I amorphous shell) have an absorption spectrum strongly resembling that of the annealed ball-milled nanoparticles (measured within minutes aer cooling to room temperature). In both of these cases, the quasi-bridging coordination binding mode is dominant (note the lack of the 1510 cm À1 absorption band). The balled-milled nanoparticles measured hours aer cooling (Fig. 4d) and the nanocubes measured aer ball-milling (Fig. 1d) show an interesting conversion of the quasi-bridging coordination binding mode (type I, amorphous shell) to the chelating coordination binding mode (type II, crystalline shell). The milling of the nanocubes introduced a surface stress, by creating a crystalline oleate shell with a chelate coordination binding mode, which was removed via annealing resulting in a transformation to a quasi-bridging coordination binding mode (Fig. 4); over time (hours) the stress/strain was reapplied as the oleate shell transformed back to the ordered chelate structure.
The condition that would allow for such a stress/strain is manifested in the nature of the type II crystalline bonding structure and the lattice structure of the BaTiO 3 core, where an epitaxial-like strain (mismatch between the shell and the core particle) is responsible for enhancing the ferroelectric properties of the nano-system, i.e. the superparticle. With the type II bond structure, a lattice mismatch exists between the crystalline shell and the core, which cannot exist with the type I amorphous shell. This is analogous to the lattice mismatch found in 2-D thin lms. 20 In order to compare the ferroelectric properties of BaTiO 3 with either a type I shell (quasi-bridging, random distribution) or a type II shell (chelating, ordered arrangement), the pre-and post-milled nanocubes are ideal samples to use as their size and shape of the core BaTiO 3 particle are practically the same (see Fig. 1 TEM images); therefore, any difference in ferroelectricity would certainly result from the carboxylate coordination binding mode. The AC displacement current density measurements (described in ref. 2, 3 and 10) of BaTiO 3 nanocubes created by solvothermal synthesis reveal a remarkable 650 times difference in magnitude of the spontaneous polarization for pre-and post-ball-milled nanocubes, P s ¼ 0.2 and P s ¼ 130 mC cm À2 , respectively. By way of comparison, the spontaneous polarization of ball-milled synthesized nanocubes is 5 times greater than that of bulk BaTiO 3 . 2 These results are very different from the cases reviewed in ref. 33. The only difference between the pre-and post-ball-milled nanocubes is the shell carboxylate coordination binding mode; this is a strong indicator that the surface strain is the mechanism behind the enhanced spontaneous polarization, and the source of the strain is indeed related to an lattice mismatch between the crystalline organic shell and core nanoparticle. Note, the milled barium oleate alone does not contribute to the enhancement of the spontaneous polarization.

Conclusions
In summary, we report on a stabilization and enhancement of spontaneous polarization in 10 nm ball-milled BaTiO 3 nanoparticles and nanocubes, which is linked to an in situ mechanochemically produced barium oleate with a crystalline chelate structure. This results in ferroelectric "hybrid" nanoparticles with an organic functional crystalline shell surrounding an inorganic core. The crystalline nature of the shell has been independently demonstrated in the results of both FTIR absorption and XRD measurements. Because of the synergistic effect of the core and the shell, this nanoparticle is described as a superparticle, where the spontaneous polarization/dipole moment belongs to the system (BaTiO 3 inorganic core and barium oleate organic shell) and not just the nanoparticle itself. 2 The mystery of the source/mechanism providing the surface stress predicted in ref. 11 has now been identied as an epitaxial-like strain between the inorganic core and the organic functional shell of the superparticle. The chelate structured carboxylate (type II shell) surrounding the core BaTiO 3 nanoparticle is the primary source of the "epitaxial" strain/stress resulting from its crystalline nature (i.e. lattice mismatch), and is not achievable using conventional wet chemistry growth techniques. Temperature dependence of the IR absorption demonstrates the effects removing the surface stress via annealing, resulting in a transformation of the chelate coordination binding mode (crystalline) to a quasi-bridging coordination binding mode (amorphous). This process is shown to be reversible with a slow transformation back to its original chelate state exhibiting a self-healing effect.
The ordered chelate carboxylate shell is responsible for a 5 times enhancement of the spontaneous polarization with respect to BaTiO 3 bulk crystal, and a 650 times enhancement of spontaneous polarization compared to synthesized (nonmilled, type I amorphous shell) unstressed BaTiO 3 nanocubes. Thus, ball-milled 10 nm BaTiO 3 nanocubes surrounded with such (type II) ligands exhibit excellent ferroelectric properties, which are relatively homogenous in shape and size. The ability to create ferroelectric nanoparticles with both a large spontaneous polarization and a uniform shape may further advance numerous elds, for example, in liquid crystal applications they would provide a means for increasing the eld sensitivity, while not introducing a plethora of defects from randomly shaped particles that could modify liquid crystal parameters such as phase behavior, transition temperatures, and long-range ordering. 34